Applied Surface Science 256 (2010) 6843–6849
Contents lists available at ScienceDirect
Applied Surface Science journal homepage: www.elsevier.com/locate/apsusc
Ammoxidation of carbon materials for CO2 capture M.G. Plaza, F. Rubiera, J.J. Pis, C. Pevida ∗ Instituto Nacional del Carbón (INCAR), CSIC, Apartado 73, 33080 Oviedo, Spain
a r t i c l e
i n f o
Article history: Received 17 March 2010 Received in revised form 23 April 2010 Accepted 25 April 2010 Available online 18 May 2010 Keywords: Ammoxidation Carbon materials Adsorption CO2 capture
a b s t r a c t Ammoxidised carbons were produced from three different starting materials: an activated carbon obtained from wood by chemical activation using the phosphoric acid process, a steam activated peatbased carbon, and a char obtained from a low-cost biomass feedstock, olive stones. Nitrogen was successfully incorporated into the carbon matrix of the different materials, the amount of nitrogen uptake being proportional to the oxygen content of the precursor. At room temperature the CO2 capture capacity of the samples was found to be related to the narrow micropore volume, while at 100 ◦ C other factors such as surface basicity took on more relevance. At 100 ◦ C all the ammoxidised samples presented an enhancement in CO2 uptake compared to the parent carbons. © 2010 Elsevier B.V. All rights reserved.
1. Introduction Carbon capture and storage (CCS) has been attracting much attention in recent years due to the urgent need to cut down greenhouse gas emissions. According to the International Energy Agency (IEA), CCS could contribute up to 19% of the cumulative effort to reduce energy-related CO2 emissions . Postcombustion capture from coal power plants has great potential for reducing CO2 emissions and the installation of several new 1400 GW coal power plants is planned before 2030 . However, postcombustion capture is faced with two difﬁcult challenges: a low CO2 partial pressure and huge volumetric ﬂow rates, which increase the cost of the separation stage. Amine scrubbing could be used as an alternative for this stage, but it has serious drawbacks, such as high energy requirements and corrosion. Adsorption has been proposed as another attractive option as it could reduce the cost associated with the capture step [3–17]. Among the adsorbents that could be used to carry out the separation of CO2 are activated carbons. These offer a number of advantages, such as ease of regeneration, low cost, high CO2 adsorption capacity, and high CO2 /N2 selectivity. Many attempts have been made to enhance the postcombustion capture performance of common adsorbents by chemically modifying their surface; among these, nitrogen enriched carbons have shown an enhancement in the CO2 capture capacity [18–25]. Nitrogen-rich carbons present other applications related to the protection of the natural environment. For instance, they have been applied to reduction of NO
∗ Corresponding author. Tel.: +34 985 11 90 90; fax: +34 985 29 76 62. E-mail address: [email protected]
(C. Pevida). 0169-4332/$ – see front matter © 2010 Elsevier B.V. All rights reserved. doi:10.1016/j.apsusc.2010.04.099
[26–28], to removal of pollutants of acidic character such as SO2 and H2 S [29,30], to adsorption of metal ions from the liquid phase , and, more recently, to the production of electrodes in electrochemical capacitors with improved performance [32,33]. Although nitrogen is not abundant in natural carbon materials, there are several ways to produce nitrogen-rich carbons: by pyrolysis of nitrogen containing polymers [23,25], by impregnation [18,19,24,34], or by reaction with ammonia [20,35–40]. Ammoxidation or the reaction of activated carbons with ammonia-air gas mixtures is another method that can be used to carry out the nitrogen enrichment of carbon materials [35–37,41–46]. In this work three different carbon materials were subjected to ammoxidation: two different types of commercial activated carbons and a char obtained in our laboratory from a low-cost biomass feedstock, olive stones. Modiﬁcation of the surface chemistry was evaluated by means of ultimate analysis, the estimation of the point of zero charge, DRIFT spectroscopy, and temperature programmed desorption tests with evolved gas analysis. The effect of ammoxidation on the texture of the samples was assessed from the N2 and CO2 adsorption isotherms at −196 and 0 ◦ C, respectively. Finally, the CO2 capture performance of the samples was determined using a thermogravimetric analyser. 2. Experimental The samples were dried overnight at 100 ◦ C prior to the ammoxidation treatment. Around 6 g of sample was placed in a quartz reactor and swept with 50 cm3 min−1 of N2 for 30 min. Then, the reactor was introduced in a vertical tube furnace, previously heated to the desired temperature. Once the sample reached that temperature, the N2 ﬂow was replaced by 50 cm3 min−1 of a gas mixture
M.G. Plaza et al. / Applied Surface Science 256 (2010) 6843–6849
containing ammonia and air at a ratio of 1:2, and held for 2 h. Afterwards, the reactor was removed from the furnace and allowed to cool down. Finally, the samples were placed in a forced air oven at 100 ◦ C for 1 h in order to desorb the weakly adsorbed ammonia. The samples were named after the starting carbon used followed by the letters NO and by the temperature of the treatment (e.g., CNO200 stands for sample C ammoxidised at 200 ◦ C). The effect of the temperature of the treatment was studied with two different types of commercial activated carbons supplied by Norit: Norit C Gran and Norit R 2030 CO2 . The ﬁrst carbon, Norit C Gran, is produced by chemical activation of wood at 550 ◦ C using the phosphoric acid process, while the second, Norit R 2030 CO2 , is a peat-based carbon activated with steam at 900 ◦ C. They will be referred to as C and R, respectively. In addition, an agricultural by-product abundant in Spain, olive stones, was selected as a low-cost feedstock for producing ammoxidised carbons. The raw stones were ground and sieved, and a particle size between 1 and 3 mm was selected for the experiments. The ﬁrst step, carbonisation, was carried out at 600 ◦ C in N2 ﬂow with an average char yield of 24%. The resulting char was denoted as O. The nitrogen uptake of the samples was determined by ultimate analysis. The change in the ratio of acidic to basic groups was evaluated from the point of zero charge (pHPZC ), determined by a mass titration method adapted from Noh and Schwarz . The modiﬁcation of the surface chemistry was also studied by DRIFT spectroscopy and temperature programmed desorption tests (TPD) together with evolved gas analysis, using a thermogravimetric analyser coupled to a FTIR spectrometer via a heated interface. The effect of ammoxidation on the porous texture of the samples was assessed from the N2 and CO2 adsorption isotherms at −196 and 0 ◦ C, respectively, obtained using a volumetric apparatus. Prior to the adsorption measurements, the samples were outgassed overnight at 100 ◦ C under vacuum. The use of both adsorbates provided complementary information. Whereas the adsorption of CO2 at 0 ◦ C and up to 1 bar is restricted to pores narrower than 1 nm, N2 adsorption at −196 ◦ C covers wider pore sizes but suffers from diffusion limitations in the narrowest pores. The apparent surface area of the samples was evaluated from the N2 adsorption isotherms by means of the BET equation (SBET ), and the total pore volume (Vp ) was assessed from the amount of nitrogen adsorbed at a relative pressure of 0.99. The micropore volume (VDR ) and narrow micropore volume (W0 ) (pore width below 0.7 nm) were estimated by applying the Dubinin–Radushkevich method to the N2 and CO2 adsorption isotherms, respectively. The mean micropore width and narrow micropore width (LDR and L0 , respectively) were calculated using the Stoeckli–Ballerini empirical relation . Finally, the CO2 capture capacity of the prepared samples was assessed using a Setaram TGA 92 thermogravimetric analyser, which recorded the mass uptake of the samples in CO2 ﬂow.
3. Results and discussion 3.1. Characterisation of the C series To select the temperature of ammoxidation, the starting carbons were subjected to temperature programmed oxidation tests at a heating rate of 15 ◦ C min−1 in 50 cm3 min−1 of air. Fig. 1 shows the corresponding TG and DTG curves of carbon C. Oxygen chemisorption takes place between 200 and 300 ◦ C, as can be seen from a slight mass gain. Above 300 ◦ C, the reactivity of the carbons in oxygen is excessively high and so 300 ◦ C was the maximum temperature studied. Table 1 presents the results of the ultimate analysis and the pHPZC of the prepared samples. Oxygen content has been calcu-
Fig. 1. Combustion proﬁle of carbon C in 50 cm3 min−1 of air ﬂow at a heating rate of 15 ◦ C min−1 .
lated by difference. Carbon C has a high oxygen content and a strong acid character due to the phosphoric acid production process. The ammoxidised samples have similar oxygen contents to the starting carbon, but signiﬁcantly higher nitrogen contents which increase with temperature: 5.0 and 9.2 wt.% at 200 and 300 ◦ C, respectively. During ammoxidation, the carbon is also oxidised, thus replacing the oxygen consumed in the reactions with ammonia . From a comparison of these results with a previous work by our group on the modiﬁcation of C by heat treatment in the presence of pure ammonia gas , it was found that nitrogen uptake is signiﬁcantly higher when the NH3 treatment is carried out in the presence of air (ammoxidation); sample C treated for 2 h with 50 cm3 min−1 of NH3 in the absence of air (amination), at 200 and 400 ◦ C, presented only 2.4 and 3.3 wt.% of N, respectively. In order to study the nature of the functionalities created by ammoxidation, the DRIFT spectra of samples C, CNO200 and CNO300, were recorded on a Nicolet Magna IR-560 spectrometer, ﬁtted with a diffuse reﬂectance accessory and a MCTA detector. 128 interferograms with a resolution of 4 cm−1 were acquired. The corresponding spectra are depicted in Fig. 2. For comparative purposes, sample CN200, obtained by amination at 200 ◦ C , has been included in this ﬁgure. The spectra of the ammoxidised samples present a band at 2225 cm−1 , which is more intense in the case of CNO300, and is ascribed to nitriles . The starting carbon, C, displays a band at 1700 cm−1 , which is characteristic of carboxyls and lactones, and a sharp band at 1600 cm−1 , related to aromatic carbon stretching with electronegative substituents (i.e., oxygen) nearby, quinones or carbonates [49,50]. If the spectra of the ammoxidised samples are compared with the spectrum of the starting carbon, it can be seen that an overlap occurs between the bands at 1600 and 1700 cm−1 . This is attributed to the formation of amides from the reaction of NH3 with surface carboxyls during ammoxidation, as Table 1 Point of zero charge and chemical analysis of the samples. Sample
C CNO200 CNO300 Rb RNO200b RNO300b O ONO300 a b
2.8 6.4 6.1 9.5 10.1 9.7 8.7 9.2
Calculated by difference. Sulfur content = 0.3 wt.%.
Ultimate analysis (wt.%, daf) C
82.9 79.2 75.0 94.7 95.7 94.4 93.0 89.2
3.0 2.5 2.0 0.4 0.1 0.2 2.2 1.9
0.4 5.0 9.2 0.7 1.0 1.7 0.3 2.6
13.7 13.3 13.8 3.9 2.9 3.4 4.5 6.3
M.G. Plaza et al. / Applied Surface Science 256 (2010) 6843–6849
Fig. 2. DRIFT spectra of samples C, CNO200, CNO300 and CN200 .
the amides absorb infrared radiation in the region between 1630 and 1680 cm−1 [35,51]. Neither nitriles nor amides were found in the CN200 spectrum. Therefore it is the presence or absence of air in the reactive atmosphere that must affect the type and amount of surface functionalities formed upon reaction with ammonia. Ammoxidation causes a shift in pHPZC (see Table 1), due to the incorporation of basic nitrogen functionalities. This increase in pHPZC is similar to that attained by amination, despite the higher nitrogen uptake achieved by ammoxidation. This is partly due to the fact that ammoxidation favours the formation of amides, which are very weak bases, as mentioned earlier. Moreover, during the amination treatment, acidic oxygen groups are consumed in the reaction with ammonia, but this time the oxygen is not replaced and so there is an increase in the pHPZC . In order to study in more detail the surface chemistry of the ammoxidised carbons, temperature programmed desorption tests were carried out at a heating rate of 15 ◦ C min−1 up to 1000 ◦ C, in 50 cm3 min−1 of Ar ﬂow rate. Fig. 3 shows the corresponding proﬁles of the evolved NH3 , HCN, CO and CO2 . NH3 emissions present two well deﬁned maxima, at 210 and 680 ◦ C. The low-temperature ammonia most probably comes from the decomposition of labile amines, while at higher temperatures it comes from the decomposition of amides and lactams [35,46]. The HCN emissions are maxima at around 730 ◦ C. These emissions arose very likely from the decomposition of nitriles, observed in the DRIFT spectra of the samples, but they may also have come from the decomposition of amides, lactams, and imides [35,46]. The ammoxidised samples present CO emissions with maxima at 665 ◦ C, outside the temperature range of the starting carbon, C. This low-temperature CO is emitted simultaneously to NH3 , so it probably originates from the decomposition of amide-like functionalities . From the CO2 proﬁles, it can also be seen that the CO2 -evolving groups (carboxyls, anhydrides and lactones) have reacted preferentially with ammonia. The bulk oxygen content does not diminish, despite the consumption of the acidic surface oxides. This is due to the simultaneous chemisorption of oxygen as CO-evolving groups, such as amides and lactams. Fig. 4 presents the N2 and CO2 adsorption isotherms of the ammoxidised samples at −196 and 0 ◦ C, respectively. The C series represents the Type IV nitrogen isotherms, with the contributions of micro- and mesoporosity. It can be observed that there is a reduction in the N2 and CO2 adsorbed volumes with increasing ammoxidation temperature. In addition, the CO2 adsorption isotherm of CNO300 shows a more pronounced curvature which indicates the narrowing of the pore width. This point is corroborated by the calculated textural parameters presented in Table 2, where it can be seen that the ammoxidation treatment reduced the porous volume of the starting carbon by narrowing the existing pores (see the decrease in LDR and L0 ). This reduction in pore volume, which becomes more pronounced with increasing temper-
Fig. 3. NH3 (a), HCN (b), CO (c) and CO2 (d) evolution proﬁles of series CNO during heating at 15 ◦ C min−1 up to 1000 ◦ C in 50 cm3 min−1 of Ar.
ature, may have been due to the surface groups introduced and to the deposition of decomposed products.
3.2. Characterisation of the R series As can be seen from Table 1, the RNO series exhibits a lower nitrogen uptake than the corresponding CNO series. This is probably due to the lower oxygen content of the R carbon. It was previously mentioned that NH3 reacted preferentially with the CO2 -evolving groups, so that R has a signiﬁcantly smaller amount of these groups (see Fig. 5). Although R was a basic carbon to begin with, it can be seen from Table 1 that the ammoxidised samples present a slightly higher pHPZC .
M.G. Plaza et al. / Applied Surface Science 256 (2010) 6843–6849
Table 2 Textural parameters and helium density of the samples. Sample
dHe (g cm−3 )
N2 adsorption at −196 ◦ C 2
SBET (m g C CNO200 CNO300 R RNO200 RNO300 O ONO300
1.51 1.56 1.61 2.14 2.14 2.13 1.65 1.62
1361 1189 964 942 999 950 43 120
CO2 adsorption at 0 ◦ C 3
Vp (cm g
0.97 0.89 0.70 0.41 0.42 0.40 0.03 0.05
VDR (cm g 0.51 0.43 0.35 0.37 0.37 0.37 – –
W0 (cm3 g−1 )
2.9 2.4 2.4 1.1 1.0 1.0 – –
0.22 0.18 0.16 0.26 0.26 0.26 0.17 0.20
0.74 0.69 0.63 0.63 0.63 0.62 0.59 0.57
mean pore width (LDR and L0 ), which is signiﬁcantly narrower than that of carbon C (cf. Table 2). 3.3. Characterisation of the biomass series The greatest nitrogen uptake was attained by the ammoxidation at 300 ◦ C of the two commercial activated carbons. For this reason, 300 ◦ C was the temperature selected for carrying out the ammoxidation of the char obtained from the olive stones. ONO300 displays a higher nitrogen and oxygen content than the starting char, O, indicating that the simultaneous chemisorption of nitrogen and oxygen took place during the ammoxidation treatment. From the shift observed in the pHPZC of the ammoxidised sample, it can be deduced that the incorporation of basic groups prevailed. Sample O aminated (treated with NH3 in the absence of air) at 400 ◦ C, exhibited a nitrogen content of 0.9 wt.% , which is signiﬁcantly lower than the 2.6 wt.% attained by ammoxidation at 300 ◦ C. Thus, the presence of air in the reactive atmosphere must promote the incorporation of nitrogen into the carbon matrix.
Fig. 4. Adsorption isotherms of N2 at −196 ◦ C (a) and CO2 at 0 ◦ C (b) for the CNO series.
The textural characterisation of the RNO series (Fig. 6) indicates that the porous system of the starting carbon, R, was virtually unaffected by the ammoxidation treatment. R is essentially microporous, with a Type I nitrogen adsorption isotherm (Fig. 6a), and a
Fig. 5. CO2 evolution proﬁles of RNO series during heating at 15 ◦ C min−1 up to 1000 ◦ C in 50 cm3 min−1 of Ar.
Fig. 6. Adsorption isotherms of N2 at −196 ◦ C (a) and CO2 at 0 ◦ C (b) for the RNO series.
M.G. Plaza et al. / Applied Surface Science 256 (2010) 6843–6849
Fig. 7. Relationship between the nitrogen uptake of the ammoxidised samples at 300 ◦ C and the oxygen content of the starting carbon material.
When the different carbons were compared, it was found that nitrogen incorporation by ammoxidation at 300 ◦ C depends very much on the oxygen content of the starting carbon (see the linear trend in Fig. 7). The TPD test of ONO300 displayed NH3 and HCN emissions (Fig. 8) with maxima at 690 and 720 ◦ C, respectively, that come from the decomposition of amides, lactams and nitriles. The shape of the NH3 and HCN proﬁles match those of the CNO series (Fig. 3), except for the absence of low-temperature NH3 from the decomposition of amines. The starting char, O, presents incipient microporosity, which is inaccessible to nitrogen molecules at −196 ◦ C, due to diffusion limitations (note that W0 is higher than Vp in Table 2). Samples O and ONO300 show narrower microporosity than carbons C and R, as can be seen from the curved shape of their CO2 adsorption isotherms (Fig. 9) and also from the mean narrow micropore width, L0 . ONO300 exhibits a higher narrow micropore volume, W0 ,
Fig. 8. NH3 (a), HCN (b) evolution proﬁles of ONO300 during heating at 15 ◦ C min−1 up to 1000 ◦ C in 50 cm3 min−1 of Ar.
Fig. 9. CO2 adsorption isotherms at 0 ◦ C of samples O and ONO300.
than the starting char, indicating that gasiﬁcation occurred to some extent during the ammoxidation treatment. However, ONO300 still suffers from N2 diffusion limitations at −196 ◦ C. 3.4. Assessment of CO2 capture capacity Fig. 10 summarises the CO2 capture capacities of the studied samples at 25 and 100 ◦ C and 1 bar. They were evaluated in a thermogravimetric analyser from the mass gain of the samples when they were exposed to 50 cm3 min−1 of CO2 . As expected, CO2 capture capacity decreases with increasing temperature. From the ﬁgure it can be seen that ammoxidation affects the CO2 capture capacity of the studied samples in different ways. In the case of carbon C, ammoxidation reduced the porous volume of the starting carbon, which might explain the decrease in the CO2 capture capacity of CNO200 and CNO300 at room temperature. However, at 100 ◦ C, sample CNO300 exhibits a CO2 capture capacity slightly higher than that of C. This may be due to its surface chemistry that plays a more active role when temperature increases. On the other hand, RNO200 and RNO300, whose texture was unaltered by ammoxidation, present a slight increase in CO2 capture capacity, which may be due to the incorporation of nitrogen functionalities. Finally, ONO300 presents a signiﬁcantly enhanced CO2 capture capacity, due to the combined effect of a higher narrow micropore volume and a favourable surface chemistry. An approximately linear relationship between the narrow micropore volume and the CO2 capture capacity of the samples can be seen in Fig. 11a. However, it should be noted that the regression coefﬁcient is signiﬁcantly better at 25 ◦ C than at 100 ◦ C. It seems that at 100 ◦ C, other parameters, such as surface basicity,
Fig. 10. CO2 capture capacities of the studied samples evaluated in a thermogravimetric analyser at 1 bar in 50 cm3 min−1 of CO2 ﬂow rate.
M.G. Plaza et al. / Applied Surface Science 256 (2010) 6843–6849
in nitrogen uptake and the type of functionalities formed by the two modiﬁcation methods. CO2 capture capacity is related to the narrow micropore volume of the samples, and this relationship is approximately linear at room temperature. However, above room temperature, the trend deviates from linearity due to the inﬂuence of other factors, such as surface basicity. Acknowledgements This work was carried out with ﬁnancial support from the Spanish MICINN (Project ENE2008-05087). M.G.P. acknowledges support from the CSIC I3P Program co-ﬁnanced by the European Social Fund. References
Fig. 11. Relationship between the CO2 capture capacity and: (a) the narrow micropore volume, W0 , and (b) the point of zero charge, pHPZC .
also inﬂuence the CO2 capture performance of the adsorbents (see Fig. 11b). The CO2 capture performance of ammoxidised samples is similar to that of the aminated samples (prepared by causing the carbons to react with dry ammonia in the absence of air) at low temperature. Sample O, aminated at 400 ◦ C, presented a CO2 capture capacity of 6.8 and 1.9 wt.% at 25 and 100 ◦ C, respectively, slightly lower than that of ONO300 (6.9 and 2.0 wt.%) . The C and R samples aminated at 200 ◦ C, displayed a CO2 capture capacity at 25 ◦ C of 6.6 and 9.2 wt.%, respectively, very close to the 6.5 and 9.2 wt.% of CNO200 and RNO200. However, better results were obtained by amination at high temperature, due to the combined effect of a suitable surface chemistry (predominance of pyridiniclike functionalities) and a higher porosity development [20,52]. 4. Conclusions It was observed that the presence or absence of air in a reactive atmosphere (ammoxidation vs. amination) signiﬁcantly affects the type and amount of surface functionalities formed upon reaction with ammonia. During ammoxidation, the formation of nitriles and amide-like functionalities is favoured and a greater amount of nitrogen is incorporated onto the carbon surface. Ammoxidation implies the simultaneous chemisorption of nitrogen and oxygen. However, nitrogen uptake by ammoxidation at 300 ◦ C was found to be proportional to the oxygen content of the starting carbon. Ammonia seems to react preferentially with the CO2 -evolving groups of the starting carbon, such as carboxyls, while the remaining oxygen mainly forms part of CO-evolving groups, such as amides or lactams. Ammoxidation treatment enhances CO2 capture to a similar extent than amination at low temperature, despite the differences
 International Energy Agency, Energy Technology Perspectives, IEA, 2008.  Q. Schiermeier, Putting the carbon back, Nature 442 (2006) 620–626.  M.T. Ho, G.W. Allinson, D.E. Wiley, Reducing the cost of CO2 capture from ﬂue gases using pressure swing adsorption, Ind. Eng. Chem. Res. 47 (2008) 4883–4890.  D. Ko, R. Siriwardane, L.T. Biegler, Optimization of pressure swing adsorption and fractionated vacuum pressure swing adsorption processes for CO2 capture, Ind. Eng. Chem. Res. 44 (2005) 8084–8094.  S.-H. Cho, J.-H. Park, H.-T. Beum, S.-S. Han, J.-N. Kim, A 2-stage PSA process for the recovery of CO2 from ﬂue gas and its power consumption, in: S.-E. Park, J.-S. Chang, K.-W. Lee (Eds.), Studies in Surface Science and Catalysis, Elsevier, 2004, pp. 405–410.  W.-K. Choi, T.-I. Kwon, Y.-K. Yeo, H. Lee, H. Song, B.-K. Na, Optimal operation of the pressure swing adsorption (PSA) process for CO2 recovery, Korean J. Chem. Eng. 20 (2003) 617–623.  J.H. Park, H.T. Beum, J.N. Kim, S.H. Cho, Numerical analysis on the power consumption of the PSA process for recovering CO2 from ﬂue gas, Ind. Eng. Chem. Res. 41 (2002) 4122–4131.  Y. Takamura, S. Narita, J. Aoki, S. Hironaka, S. Uchida, Evaluation of dual-bed pressure swing adsorption for CO2 recovery from boiler exhaust gas, Sep. Purif. Technol. 24 (2001) 519–528.  M. Ishibashi, H. Ota, N. Akutsu, S. Umeda, M. Tajika, J. Izumi, A. Yasutake, T. Kabata, Y. Kageyama, Technology for removing carbon dioxide from power plant ﬂue gas by the physical adsorption method, Energy Convers. Manage. 37 (1996) 929–933.  G.D. Pirngruber, S. Cassiano-Gaspar, S. Louret, A. Chaumonnot, B. Delfort, Amines immobilized on a solid support for postcombustion CO2 capture—a preliminary analysis of the performance in a VSA or TSA process based on the adsorption isotherms and kinetic data, Energy Procedia 1 (2009) 1335– 1342.  J. Zhang, P.A. Webley, P. Xiao, Effect of process parameters on power requirements of vacuum swing adsorption technology for CO2 capture from ﬂue gas, Energy Convers. Manage. 49 (2008) 346–356.  A.L. Chaffee, G.P. Knowles, Z. Liang, J. Zhang, P. Xiao, P.A. Webley, CO2 capture by adsorption: materials and process development, Int. J. Greenh. Gas Con. 1 (2007) 11–18.  N. Tlili, G. Grévillot, C. Vallières, Carbon dioxide capture and recovery by means of TSA and/or VSA, Int. J. Greenh. Gas Con. 3 (2009) 519–527.  J. Merel, M. Clausse, F. Meunier, Experimental investigation on CO2 postcombustion capture by indirect thermal swing adsorption using 13X and 5A zeolites, Ind. Eng. Chem. Res. 47 (2008) 209–215.  C.A. Grande, R.P.P.L. Ribeiro, A.E. Rodrigues, CO2 capture from NGCC power stations using electric swing adsorption (ESA), Energy Fuel 23 (2009) 2797– 2803.  C.A. Grande, A.E. Rodrigues, Electric swing adsorption for CO2 removal from ﬂue gases, Int. J. Greenh. Gas Con. 2 (2008) 194–202.  M. Radosz, X. Hu, K. Krutkramelis, Y. Shen, Flue-gas carbon capture on carbonaceous sorbents: toward a low-cost multifunctional carbon ﬁlter for “green” energy producers, Ind. Eng. Chem. Res. 47 (2008) 3783–3794.  M.M. Maroto-Valer, Z. Lu, Y. Zhang, Z. Tang, Sorbents for CO2 capture from high carbon ﬂy ashes, Waste Manage. 28 (2008) 2320–2328.  M.M. Maroto-Valer, Z. Tang, Y. Zhang, CO2 capture by activated and impregnated anthracites, Fuel Process. Technol. 86 (2005) 1487–1502.  C. Pevida, M.G. Plaza, B. Arias, J. Fermoso, F. Rubiera, J.J. Pis, Surface modiﬁcation of activated carbons for CO2 capture, Appl. Surf. Sci. 254 (2008) 7165– 7172.  J. Przepiórski, M. Skrodzewicz, A.W. Morawski, High temperature ammonia treatment of activated carbon for enhancement of CO2 adsorption, Appl. Surf. Sci. 225 (2004) 235–242.  C. Pevida, C.E. Snape, T.C. Drage, Templated polymeric materials as adsorbents for the postcombustion capture of CO2 , Energy Procedia 1 (2009) 869–874.  C. Pevida, T.C. Drage, C.E. Snape, Silica-templated melamine-formaldehyde resin derived adsorbents for CO2 capture, Carbon 46 (2008) 1464–1474.
M.G. Plaza et al. / Applied Surface Science 256 (2010) 6843–6849  M.G. Plaza, C. Pevida, A. Arenillas, F. Rubiera, J.J. Pis, CO2 capture by adsorption with nitrogen enriched carbons, Fuel 86 (2007) 2204–2212.  T.C. Drage, A. Arenillas, K.M. Smith, C. Pevida, S. Piippo, C.E. Snape, Preparation of carbon dioxide adsorbents from the chemical activation of urea-formaldehyde and melamine-formaldehyde resins, Fuel 86 (2007) 22–31.  M.-C. Huang, H. Teng, Nitrogen-containing carbons from phenol-formaldehyde resins and their catalytic activity in NO reduction with NH3 , Carbon 41 (2003) 951–957.  T. Grzybek, J. Klinik, B. Samojeden, V. Suprun, H. Papp, Nitrogen-promoted active carbons as denox catalysts. 1. The inﬂuence of modiﬁcation parameters on the structure and catalytic properties, Catal. Today 137 (2008) 228–234.  C. Pevida, A. Arenillas, F. Rubiera, J.J. Pis, Heterogeneous reduction of nitric oxide over synthetic coal chars, Fuel 84 (2005) 2275–2279.  J.P. Boudou, M. Chehimi, E. Broniek, T. Siemieniewska, J. Bimer, Adsorption of H2 S or SO2 on an activated carbon cloth modiﬁed by ammonia treatment, Carbon 41 (2003) 1999–2007.  J. Bimer, P.D. Salebut, S. Berleo zecki, J.P. Boudou, E. Broniek, T. Siemieniewska, Modiﬁed active carbons from precursors enriched with nitrogen functions: sulfur removal capabilities, Fuel 77 (1998) 519–525.  S. Biniak, M.G. Pakulea, S. Szymanski, A. Swiatkowski, Effect of activated carbon surface oxygen- and/or nitrogen-containing groups on adsorption of copper(II) ions from aqueous solution, Langmuir 15 (1999) 6117–6122.  R. Pietrzak, K. Jurewicz, P. Nowicki, K. Babel, H. Wachowska, Microporous activated carbons from ammoxidised anthracite and their capacitance behaviours, Fuel 86 (2007) 1086–1092.  K. Jurewicz, R. Pietrzak, P. Nowicki, H. Wachowska, Capacitance behaviour of brown coal based active carbon modiﬁed through chemical reaction with urea, Electrochim. Acta 53 (2008) 5469–5475.  M.L. Gray, Y. Soong, K.J. Champagne, J. Baltrus, R.W. Stevens Jr., P. Toochinda, S.S.C. Chuang, CO2 capture by amine-enriched ﬂy ash carbon sorbents, Sep. Purif. Technol. 35 (2004) 31–36.  R.J.J. Jansen, H. van Bekkum, Amination and ammoxidation of activated carbons, Carbon 32 (1994) 1507–1516.  R. Pietrzak, XPS study and physico-chemical properties of nitrogen-enriched microporous activated carbon from high volatile bituminous coal, Fuel 88 (2009) 1871–1877.  R. Pietrzak, H. Wachowska, P. Nowicki, K. Babel, Preparation of modiﬁed active carbon from brown coal by ammoxidation, Fuel Process. Technol. 88 (2007) 409–415.
 C.L. Mangun, K.R. Benak, J. Economy, K.L. Foster, Surface chemistry, pore sizes and adsorption properties of activated carbon ﬁbers and precursors treated with ammonia, Carbon 39 (2001) 1809–1820.  P Vinke, M. van der Eijk, M. Verbree, A.F. Voskamp, H. van Bekkum, Modiﬁcation of the surfaces of a gas activated carbon and a chemically activated carbon with nitric acid, hypochlorite, and ammonia, Carbon 32 (1994) 675–686.  G.M.K. Abotsi, A.W. Scaroni, Reaction of carbons with ammonia: effects on the surface charge and molybdenum adsorption, Carbon 28 (1990) 79–84.  L. Wachowski, M. Hofman, Application of TG–DTG analysis in the study of the ammoxidised carbon materials, J. Therm. Anal. Calorim. 83 (2006) 379–383.  K. Jurewicz, K. Babel, R. Pietrzak, S. Delpeux, H. Wachowska, Capacitance properties of multi-walled carbon nanotubes modiﬁed by activation and ammoxidation, Carbon 44 (2006) 2368–2375.  K. Jurewicz, K. Babel, A. Ziólkowski, H. Wachowska, Capacitance behaviour of the ammoxidised coal, J. Phys. Chem. Solids 65 (2004) 269–273.  K. Jurewicz, K. Babel, A. Ziólkowski, H. Wachowska, Ammoxidation of active carbons for improvement of supercapacitor characteristics, Electrochim. Acta 48 (2003) 1491–1498.  K. Jurewicz, K. Babel, A. Ziólkowski, H. Wachowska, M. Kozlowski, Ammoxidation of brown coals for supercapacitors, Fuel Process. Technol. 77–78 (2002) 191–198.  R.J.J. Jansen, H. van Bekkum, XPS of nitrogen-containing functional groups on activated carbon, Carbon 33 (1995) 1021–1027.  J.S. Noh, J.A. Schwarz, Estimation of the point of zero charge of simple oxides by mass titration, J. Colloid Interf. Sci. 130 (1989) 157–164.  F. Stoeckli, L. Ballerini, Evolution of microporosity during activation of carbon, Fuel 70 (1991) 557–559.  P.E. Fanning, M.A. Vannice, A DRIFT study of the formation of surface groups on carbon by oxidation, Carbon 31 (1993) 721–730.  J.L. Figueiredo, M.F.R. Pereira, M.M.A. Freitas, J.J.M. Órfão, Modiﬁcation of the surface chemistry of activated carbons, Carbon 37 (1999) 1379–1389.  B. Stohr, H.P. Boehm, R. Schlogl, Enhancement of the catalytic activity of activated carbons in oxidation reactions by thermal treatment with ammonia or hydrogen cyanide and observation of a superoxide species as a possible intermediate, Carbon 29 (1991) 707–720.  M.G. Plaza, C. Pevida, B. Arias, J. Fermoso, M.D. Casal, C.F. Martín, F. Rubiera, J.J. Pis, Development of low-cost biomass-based adsorbents for postcombustion CO2 capture, Fuel 88 (2009) 2442–2447.